SURFACE SLURRY SEALING SYSTEMS IN CANADA:
PERFORMANCE AND PRACTICE
JEAN-MARTIN CROTEAU, P.Eng.Miller Paving Limited
J. KEITH DAVIDSON, P. Eng.McAsphalt Engineering Services
PETER PERRONEMcAsphalt Industries Limited
434 SLURRY SEALING - PERFORMANCE AND PRACTICE
Traditional slurry seal systems were first used in Canada in the 1960s while polymer-modified systemswere introduced in the early 1990s. Surface slurry sealing systems are placed to restore the surfacecharacteristics of pavement or to preserve a pavement. The systems can be designed to correct rutting, toimprove skid resistance, to seal and to protect the pavement surface. Skid Numbers for surface slurrysealing systems can reach the 50s, which, in terms of skid resistance, is exceptionally good. They can beapplied on chip seals, on hot mix asphalt pavement or on concrete pavement.
Surface slurry sealing systems are mixtures of cationic emulsified asphalt, mineral aggregates, mineralfiller, water and additives, properly proportioned, mixed and spread with a machine over a properlyprepared surface. A slurry mixture forms an impervious thin overlay over an existing pavement. The rateof application ranges from approximately 8.0 kg/m for a non-polymer modified fine graded system to 18kg/m for a polymer coarse graded system.
This paper presents an overview of the surface slurry sealing systems technology and a discussion on thestate of the practice including design practices, construction procedures and the performance of thesesurface treatments.
Les systmes traditionnels de coulis de scellement ont t utiliss pour la premire fois dans les annes1960 alors que les systmes modifis au polymre ont t introduits dans les annes 1990. Les systmesde coulis de scellement de surface sont poss pour restaurer les caractristiques de surface de la chausseou pour prserver une chausse. Les systmes peuvent tre conus pour corriger lornirage, amliorer larsistance la glissance, sceller et protger la surface de la chausse. Les donnes de glissance duncoulis de scellement de surface peuvent atteindre les 50, ce qui, en termes de rsistance la glissance, estexceptionnellement bon. Ils peuvent tre appliqus sur des enduits superficiels, sur des chausses enenrobs bitumineux chaud ou en bton de ciment.
Les systmes de coulis de scellement de surface sont des mlanges dmulsion cationique de bitume, degranulats, de filler minral, deau et dadditifs bien proportionns, malaxs et pandus avec une machinesur une surface correctement prpare. Un mlange de coulis forme un revtement mince sans vide surune chausse existante. Le taux dapplication varie denviron 8,0 kg/m2 pour un systme granulomtriefine sans polymre 18 kg/m2 pour un systme granulomtrie grossire avec polymre.
Cet expos prsente une vue gnrale de la technologie des systmes de coulis de scellement de surface etune discussion sur ltat de la pratique incluant les usages de design, les procds de construction et laperformance de ces traitements de surface.
CROTEAU, DAVIDSON & PERRONE 435
Surface slurry sealing systems have been used in Canada for many years. Traditional non-polymermodified slurry seal systems were used for the first time in the 1960s, while the polymer-modified micro-surfacing systems were introduced in Canada in the early 1990s. It is estimated that approximately 3.5million square meters of slurry surfacing systems are placed every year in Canada. Surface slurry sealingsystems are used to restore the surface characteristics of pavement or as a pavement preservationtreatment. The usage of surface slurry systems is increasing in nearly every province in Canada. Thispaper presents an overview of the surface slurry sealing systems technology and a discussion on the stateof the practice including, design practices, construction procedures and the performance of these surfacetreatments.
The first form of slurry surfacing can be traced back to the late 1920s with a process call schlmme.The schlmme process was developed in Germany and it consisted of mixing a hot bituminous binderwith a very fine aggregate and water. The schlmme mixture was prepared in a central plant,maintained under agitation during transportation to avoid sedimentation and placed using brushes andrubber scrapers. After the evaporation of water, the finished product was smooth and waterproof.
The hot bituminous binder was eventually replaced with a slow setting anionic emulsion. The slurrymixture was prepared, transported and placed in the same manner as the schlmme process. It was notuntil the 1960s, with the development of cationic emulsions and continuous flow lay down machines, thata strong interest in using slurry surfacing for road maintenance started. The break of the newly developedcationic emulsions was better controlled and not as dependent on the weather conditions. The trafficreadiness of the cationic type slurry seal surfacing was reduced from several hours to one or two hours.The development of continuous flow lay down machines also allowed the placement of slurry surfacingover large areas in a short period of time.
The first polymer-modified slurry sealing system was developed in Germany in the late 1970s. Polymer-modified systems, also called micro-surfacing, are composed of polymer-modified cationic emulsion,crushed aggregates, mineral filler, water and field control additives. The first system was commercializedunder the trade name Ralumac and it was imported into North America in the early 1980s. Today severalother proprietary and generic systems are available in North America and abroad. The most common usesof micro-surfacing are surface texturing, surface sealing and rut filling of bituminous pavement.
Surface slurry sealing systems include different processes that ought to be differentiated.
Quickset Slurry Seals: Quickset slurry seals are mainly used as sealants on bituminous pavement. Theaggregate is relatively fine (less than 6.3 mm) and always 100 % crushed. The emulsion is not modifiedand always cationic. The fines content ranges between 8 to 12 % and the residual bituminous binder isgenerally between 9.0 and 10 %. The application rate for a typical bituminous pavement ranges between6.5 and 7.0 kg/m2.
Polymer-modified Quickset Slurry Seals: Polymer-modified quickset slurry seals are also used assealants on bituminous pavement. They are formulated in the same manner as traditional quickset slurry
436 SLURRY SEALING - PERFORMANCE AND PRACTICE
seals with the exception that the emulsion is modified with a low loading of polymer, about 1.0 %. Thisallows the slurry to be applied at a slightly higher rate, which ranges between 7.5 and 9.5 kg/m2.
Micro-Surfacing: Micro-surfacing systems are used not only as sealants but also for surface texturingand rut filling of pavement. The maximum size of the aggregate is greater than the maximum size of theaggregate used for slurry seal. The maximum size of the aggregate is between 6.3 and 9.5 mm and it isalways 100 % crushed. The emulsion is modified with a heavy polymer loading, between 3.0 and 4.0 %,and the emulsion is always cationic. The fines content ranges between 7 to 10 % and the residualbituminous binder is generally between 8.0 and 9.0 %. The application rate for a typical bituminouspavement ranges between 12.0 and 18.0 kg/m2.
Fiber Modified Micro-Surfacing: Fiber modified micro-surfacing systems were developed in Europeand they are not yet commonly used in North America. They were developed to provide a very aggressivemacro-texture to the surface of the pavement. The aggregate is often gap graded and the fiber loadinghelps to prevent segregation. With the exception of the fibers and the gradation of the aggregate, fibermodified micro-surfacing is formulated in the same manner as traditional micro-surfacing.
Contrary to a wide spread perception, the fundamental difference between the slurry seal systems and themicro-surfacing systems is not associated with the type of emulsion used to produce the slurry mixture. Itis related to the tightness and strength of the mineral skeleton in the aggregate/bitumen matrix once thewater escapes. Micro-surfacing is formulated in such a manner that once the water escapes the mineralparticles are interlocked and the mineral skeleton is strong. Hence it is possible to place micro-surfacingmaterial in thick lifts or in multiple layers without risk of deformation. Slurry seal systems are formulatedwith the objective of creating a bitumen rich mortar. The mineral skeleton is not very strong and there isminimal interlocking of the aggregate particles. Consequently, the thickness at which slurry seal systemscan be place is limited because there is a risk of deformation.
2. SLURRY MIXTURE
The formulation of a slurry mixture is carried out in three stages as described below:- component selection and testing to determine whether they are suitable and meet the
materials specification,- mixture testing to confirm that the two main components, i.e., the emulsion and the mineral
aggregate are compatible and to determine the effect of the water, the filler and the fieldcontrol additives
- performance testing to determine the optimum slurry mixture formulation
2.1 Components Selection and Testing
The first step in the process of establishing a slurry mixture formulation is the selection and testing of thevarious components which include: aggregate, mineral filler, fibers (if required), added water, emulsionand field control additives.
The aggregate constitutes about 82 to 90 % by weight of the slurry mixture, depending on the aggregatenatur